Thermo- and light-triggered reversible interconversion of dysprosium-anthracene complexes and their responsive optical, magnetic and dielectric properties.
Huang, Xin-Da; Wen, Ge-Hua; Bao, Song-Song; Jia, Jia-Ge; Zheng, Li-Min; Chemical science 12 (2020) 929–937; doi:10.1039/d0sc04851h

data_1559657
_publ_section_title
;
 Thermo- and light-triggered reversible interconversion of
 dysprosium-anthracene complexes and their responsive optical, magnetic
 and dielectric properties.
;
_journal_issue                   3
_journal_name_full               'Chemical science'
_journal_page_first              929
_journal_page_last               937
_journal_paper_doi               10.1039/d0sc04851h
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety         'C51 H52 Dy N5 O8 P2 S3'
_chemical_formula_sum            'C51 H52 Dy N5 O8 P2 S3'
_chemical_formula_weight         1183.59
_chemical_name_systematic        1LT
_chemical_properties_physical    Photo-sensitive
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2020-07-07 deposited with the CCDC.	2020-11-11 downloaded from the CCDC.
;
_cell_angle_alpha                90.03(7)
_cell_angle_beta                 91.86(4)
_cell_angle_gamma                112.38(7)
_cell_formula_units_Z            2
_cell_length_a                   9.592(14)
_cell_length_b                   11.701(19)
_cell_length_c                   26.20(4)
_cell_measurement_reflns_used    5671
_cell_measurement_temperature    193(2)
_cell_measurement_theta_max      27.297
_cell_measurement_theta_min      2.3275
_cell_volume                     2717(7)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT 2014/4 (Sheldrick, 2014)'
_diffrn_ambient_temperature      193(2)
_diffrn_measured_fraction_theta_full 0.981
_diffrn_measured_fraction_theta_max 0.968
_diffrn_measurement_device_type  'Bruker D8 Venture'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0665
_diffrn_reflns_av_unetI/netI     0.1291
_diffrn_reflns_Laue_measured_fraction_full 0.981
_diffrn_reflns_Laue_measured_fraction_max 0.968
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -33
_diffrn_reflns_number            19335
_diffrn_reflns_point_group_measured_fraction_full 0.981
_diffrn_reflns_point_group_measured_fraction_max 0.968
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.183
_diffrn_reflns_theta_min         1.882
_exptl_absorpt_coefficient_mu    1.604
_exptl_absorpt_correction_T_max  0.740
_exptl_absorpt_correction_T_min  0.733
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS 2016/2'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    1.447
_exptl_crystal_description       block
_exptl_crystal_F_000             1202
_exptl_crystal_preparation       'Magnetic properties,Luminescent,Dielectric'
_exptl_crystal_recrystallization_method 'Vapour deposition'
_exptl_crystal_size_max          0.200
_exptl_crystal_size_mid          0.200
_exptl_crystal_size_min          0.200
_refine_diff_density_max         3.351
_refine_diff_density_min         -3.027
_refine_diff_density_rms         0.194
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.087
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     635
_refine_ls_number_reflns         11705
_refine_ls_number_restraints     426
_refine_ls_restrained_S_all      1.076
_refine_ls_R_factor_all          0.1557
_refine_ls_R_factor_gt           0.1088
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0534P)^2^+63.5785P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2531
_refine_ls_wR_factor_ref         0.2777
_reflns_Friedel_coverage         0.000
_reflns_number_gt                7884
_reflns_number_total             11705
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d0sc04851h2.cif
_cod_data_source_block           1LT
_cod_depositor_comments
;Adding full bibliography for 1559656--1559657.cif.

 Adding full bibliography for 1559656--1559657.cif.
;
_cod_original_cell_volume        2717(8)
_cod_database_code               1559657
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_min   0.740
_shelx_estimated_absorpt_t_max   0.740
_shelx_res_checksum              67190